- Email: [email protected]

Contents lists available at ScienceDirect

Journal of Luminescence journal homepage: www.elsevier.com/locate/jlumin

Built-in electric ﬁeld effect on the linear and nonlinear intersubband optical absorptions in InGaN strained single quantum wells Yue-meng Chi, Jun-jie Shi State Key Laboratory for Mesoscopic Physics and Department of Physics, Peking University, Beijing 100871, PR China

a r t i c l e in f o

a b s t r a c t

Article history: Received 3 January 2007 Received in revised form 8 April 2008 Accepted 5 May 2008 Available online 14 May 2008

Considering the strong built-in electric ﬁeld (BEF) induced by the spontaneous and piezoelectric polarizations and the intrasubband relaxation, we investigate the linear and nonlinear intersubband optical absorptions in Inx Ga1x N/Aly Ga1y N strained single quantum wells (QWs) by means of the density matrix formalism. Our numerical results show that the strong BEF is on the order of MV/cm, which can be modulated effectively by the In composition in the QW. This electric ﬁeld greatly increases the electron energy difference between the ground and the ﬁrst excited states. The electron wave functions are also signiﬁcantly localized in the QW due to the BEF. The intersubband optical absorption peak sensitively depends on the compositions of In in the well layer and Al in the barrier layers. The intersubband absorption coefﬁcient can be remarkably modiﬁed by the electron concentration and the incident optical intensity. The group-III nitride semiconductor QWs are suitable candidate for infrared photodetectors and near-infrared laser ampliﬁers. & 2008 Elsevier B.V. All rights reserved.

PACS: 73.21.Fg 77.65.Ly 77.84.Bw Keywords: InGaN quantum wells Built-in electric ﬁeld Linear and nonlinear intersubband optical absorptions

1. Introduction During the last couple of years, group-III nitride semiconductors have attracted much attention as materials for high-brightness light emitting diodes and laser diodes [1,2]. Such devices operate on the basis of the band to band (interband) transitions. However, due to the large conduction band offset, the III-nitride semiconductors low-dimensional heterostructures can also be designed to have transitions between the conduction subbands (intersubbands) with energy spacing in the near-infrared region [3,4]. Recently, the intersubband optical transition in III-nitride semiconductor quantum heterostructures has attracted much attention [5,6]. The ternary compound semiconductor heterostructures, such as InGaN/GaN, InGaN/AlGaN and GaN/AlGaN quantum wells (QWs), are all good candidates for some important optoelectronic devices, such as infrared photodetectors and waveguide switches working in the near-infrared range. Hence the intersubband optical transition in low-dimensional semiconductor heterostructures has always been a hot topic from both experiments [7–9] and theories [10,11] in recent years. In the present paper, we pay much attention to InGaN/AlGaN QWs.

Corresponding author. Tel.: +86 10 62757594; fax: +86 10 62751615.

E-mail address: [email protected] (J.-j. Shi). 0022-2313/$ - see front matter & 2008 Elsevier B.V. All rights reserved. doi:10.1016/j.jlumin.2008.05.006

The group-III nitride semiconductors have large piezoelectric constants along the [0 0 0 1] direction [12]. Considering the strain of the wurtzite InGaN/AlGaN double heterostructure due to large lattice mismatch, the spontaneous and piezoelectric polarizations of the structure [13] can give rise to large polarization sheet charges on the interfaces or surfaces of the system, which, in turn, create a deﬁnite internal built-in electric ﬁeld (BEF) inside the heterostructure. The intensity of the BEF can be estimated on the order of MV/cm [14] (see Fig. 1). A large dipole strength due to the BEF has been calculated [15]. It suggests that the intersubband optical transitions in the InGaN QWs have very large optical nonlinearity. These linear and nonlinear size-quantized intersubband optical transitions are interesting both for the fundamental investigation and for device applications, such as near-infrared laser ampliﬁers, photodetectors and high-speed electrooptical modulators [3,4,7]. To the best of our knowledge, there is little investigation for the linear and nonlinear intersubband optical absorptions in the important III-nitride QWs due to the strong BEF effect. The paper is organized as follows. In Section 2, the BEF due to the piezoelectric and spontaneous polarizations in the InGaN/ AlGaN strained QWs is calculated. In Section 3, the electron states conﬁned in InGaN/AlGaN strained QWs are solved. In Section 4, the theoretical framework of the linear and nonlinear intersubband optical absorptions in the InGaN/AlGaN QWs is outlined. Numerical results for the intersubband optical

ARTICLE IN PRESS Y.-m. Chi, J.-j. Shi / Journal of Luminescence 128 (2008) 1836–1840

1837

where F n (n ¼ Inx Ga1x N or Aly Ga1y N) denotes the BEF of layer n and is caused by polarization of the QW structure, and ene is the electronic dielectric constant of the material n. Based on Eq. (3) and the boundary condition that the potential energies on the far left and right of the QW structure are the same, we can obtain F

InGaN

PInGaN þ P InGaN P AlGaN SP PE SP ¼ eInGaN e0 e

F AlGaN ! 0

Fig. 1. Magnitude of the built-in electric ﬁeld in the InGaN layer along the c axis as a function of the In composition for strained Inx Ga1x N=Al0:2 Ga0:8 N QW with the well width LInGaN ¼ 2 nm.

(4)

In general, the direction of the BEF in the InGaN layer depends on the orientation of the piezoelectric and spontaneous polarizations and can be determined by both the polarity of the crystal and the strain of the QW structure. For our Aly Ga1y N=Inx Ga1x N/Aly Ga1y N strained single QW, the direction of the BEF is along the z-direction. Based on Eq. (4), we have calculated the strength of F InGaN in the strained Inx Ga1x N layer as a function of In composition. We can ﬁnd from Fig. 1 that the BEF is extremely

absorptions are given and discussed in Section 5. Finally, we summarize the main conclusions obtained in this paper in Section 6.

2. BEF in strained group III nitride QWs It has been known that both Inx Ga1x N and Aly Ga1y N are wurtzite crystal structure, in which the chemical bonds between the neighboring atoms are not equivalent. This directly leads to a strong spontaneous polarization along the [0 0 0 1] direction [16]. The wurtzite crystal structure has also been found to have three independent nonvanishing component (e31 ; e33 ; e15 ) of the piezoelectric tensor [16]. Therefore, the total zero-ﬁeld macroscopic ! ! polarization P tot includes both the spontaneous polarization P SP in the equilibrium lattice and the strain-induced or piezoelectric ! polarization P PE . For simplicity, we consider an Inx Ga1x N/Aly Ga1y N strained single QW with a thin Inx Ga1x N layer sandwiched between two thick Aly Ga1y N layers grown along the [0 0 0 1] direction (caxis) of the bulk materials denoted as the z direction. Following Takeuchi et al. [17], we ignore the complicated strains of the thick AlGaN layers due to the lattice and thermal mismatch of AlGaN and substrate (sapphire or SiC). The lattice constant a of the InGaN layer is reduced and c increased because of biaxial compressive stress. The total zero-ﬁeld macroscopic polarization in the thick AlGaN layer is given by !AlGaN !AlGaN P tot z^ ¼ P SP ¼ P AlGaN SP

(1)

The total zero-ﬁeld macroscopic polarization in the thin InGaN strained layer can be expressed as !InGaN !InGaN !InGaN P tot ¼ P SP þ P PE ¼ P InGaN z^ þ ½e31 ðexx þ eyy Þ þ e33 ezz z^ SP

(2)

Here exx , eyy , and ezz are the strain elements of the InGaN strained layer. Considering the continuity of the electric displacement vector at the heterointerfaces of semiconductor QWs, we have eAlGaN e0 F AlGaN eInGaN e0 F InGaN e e ¼ P InGaN þ PInGaN P AlGaN SP PE SP

(3)

Fig. 2. Schematic diagrams of wave functions for an electron conﬁned in a strained Inx Ga1x N/Aly Ga1y N QW with the two heterointerfaces located at z ¼ 5 and 5 nm, respectively. Here the strong built-in electric ﬁeld is included in (a) and ignored in (b).

ARTICLE IN PRESS 1838

Y.-m. Chi, J.-j. Shi / Journal of Luminescence 128 (2008) 1836–1840

strong, of the order of MV/cm. The increase of the In composition will enlarge the magnitude of the BEF in the InGaN strained layer. Moreover, we can see from Fig. 2 that the strong BEF in the strained Inx Ga1x N/Aly Ga1y N QW can induce a remarkable change of the electron wave function spatial distribution. The electron wave functions are pushed to the right side of the QW, and the electrons are localized in the vicinity of the right interface of the QW due to the BEF. Moreover, we can also ﬁnd from Fig. 2 that, compared with the case of ignoring the BEF, the energy separation between the ground and the ﬁrst excited states increases if the BEF is included. The intersubband optical absorption peak will thus be signiﬁcantly blue shifted by the BEF (refer to Fig. 4).

3. Electron states in strained InGaN single QWs Let us now consider an electron conﬁned in an Inx Ga1x N/Aly Ga1y N symmetric single QW with a well width L. Within the framework of the effective mass approximation, the electron Hamiltonian in the z direction can be written as 2

2 ^ ¼ _ d þ VðzÞ eFz H 2m dz2

(5)

where m and e denote the electron effective mass and the absolute value of the electron charge, respectively. VðzÞ is the electron conﬁned potential in the QW,

functions Ai and Bi, 8 kL ðzþL=2Þ ; > < fBiðt L Þ lAiðt L Þg e cðzÞ ¼ BiðtÞ lAiðtÞ; > : fBiðt Þ lAiðt Þg ekR ðzL=2Þ ; R

R

zp L=2 jzjoL=2

(13)

zXL=2

where KBi0 ðt L Þ þ kL Biðt L Þ KAi0 ðt L Þ þ kL Aiðt L Þ 1=3 2m E t¼ eF z þ eF _2

l¼

(14) (15)

4. Linear and nonlinear intersubband optical absorptions in strained InGaN single QWs By means of the density matrix method [18,19], the linear and nonlinear intersubband optical absorption coefﬁcients in an Inx Ga1x N/Aly Ga1y N strained QW can be derived as?A3B2 tptxt=10pt?> rﬃﬃﬃﬃﬃ m m kB T jM21 j2 að1Þ ðoÞ ¼ o R Lp_2 1 þ exp½ðEF E1 Þ=kB T ln 1 þ exp½ðEF E2 Þ=kB T _=tin (16) ðE2 E1 _oÞ2 þ ð_=tin Þ2 and

rﬃﬃﬃﬃﬃ m I m kB T að3Þ ðo; IÞ ¼ o 2 R 20 nr c Lp_ 1 þ exp½ðEF E1 Þ=kB T ln 1 þ exp½ðEF E2 Þ=kB T

jM 21 j2 ð_=tin Þ

½ðE2 E1 _oÞ2 þ ð_=tin Þ2 2 " # jM 22 M11 j2 fðE2 E1 _oÞ2 ð_=tin Þ2 þ 2ðE2 E1 ÞðE2 E1 _oÞg 4jM 21 j2 ðE2 E1 Þ2 þ ð_=tin Þ2 ( VðzÞ ¼

V 0;

jzj4L=2

0;

jzjpL=2

(6)

Here V 0 is the potential height between Inx Ga1x N and Aly Ga1y N, which can be determined by the band-gap discontinuity DEG. F in Eq. (5) is the absolute value of the BEF in the strained QW, which can be calculated from Eq. (4). The electron bound state energy E can be obtained by solving ½kR Aiðt R Þ KAi0 ðt R Þ ½kL Biðt L Þ þ KBi0 ðt L Þ ¼ ½kL Aiðt L Þ þ KAi0 ðt L Þ ½kR Biðt R Þ KBi0 ðt R Þ

(7)

where 1=3 2m E L eF tL ¼ eF 2 _2 1=3 2m E L tR ¼ þ eF eF 2 _2 1=2 2m eFL E kL ¼ V þ 0 2 _2 1=2 2m eFL E V kR ¼ 0 2 _2 1=3 2m eF K¼ _2

(17)

where m is the permeability of the well material, R is the real part of the permittivity, nr is the refractive index (R ¼ n2r 0 ), c is the speed of light in free space, E1 ðE2 Þ is the initial (ﬁnal) state energy, tin is the intrasubband relaxation time, o is the angular frequency of optical radiation, I is the optical intensity, and EF is the Fermi energy. It is worthwhile to point out that the linear absorption comes from the contribution of the linear susceptibility wð1Þ term and the nonlinearity in the absorption coefﬁcient is due to the third-order nonlinear susceptibility wð3Þ term [20]. For an intersubband optical transition with polarization along z direction, the dipole matrix element can be written as Mij ¼ hije zjji

(18)

(8) (9)

where jii and jji denote initial and ﬁnal states of the optical transition, respectively. Based on Eqs. (16) and (17), the total intersubband optical absorption coefﬁcient aðo; IÞ can be given by

(10)

aðo; IÞ ¼ að1Þ ðoÞ þ að3Þ ðo; IÞ

(11)

Since að3Þ ðo; IÞ is negative and is proportional to the intensity I, aðo; IÞ decreases as I increases. The absorption coefﬁcient aðo; IÞ is reduced by one-half when I reaches a value Is called the saturation intensity [20], so we have the following relation:

(12)

The electron wave function in the z direction cðzÞ can be obtained by means of a linear combination of the two independent Airy

aðo; Is Þ ¼ að1Þ ðoÞ=2

(19)

(20)

ARTICLE IN PRESS Y.-m. Chi, J.-j. Shi / Journal of Luminescence 128 (2008) 1836–1840

1839

or equivalently, að3Þ ðo; Is Þ ¼ að1Þ ðoÞ=2

(21)

5. Numerical results and discussion We have solved the electron states and calculated the linear and nonlinear intersubband optical absorption coefﬁcients for Inx Ga1x N/Aly Ga1y N strained single QWs. The physical parameters are chosen as follows. The electron effective mass is m ¼ 0:2m0 [21]. The real part of the permittivity is chosen to be R ¼ 10:4 [21]. The lattice constants are a ¼ 3:189ð1 xÞ þ 3:548x A for Inx Ga1x N [21], and a ¼ 3:189ð1 yÞ þ 3:112y A for Aly Ga1y N [22]. The band-gap discontinuity is DEG ¼ f3:4ð1 yÞ þ 6:2y yð1 yÞg f3:4ð1 xÞ þ 1:9x 3:2xð1 xÞg eV [17,21,22]. The conduction band offset is chosen as 75% of the total band-gap discontinuity [23]. The spontaneous polarizations are P InGaN ¼ SP 0:029ð1 xÞ 0:032x C=m2 for Inx Ga1x N and P AlGaN ¼ 0:029 SP ð1 yÞ 0:081y C=m2 for Aly Ga1y N [22]. The piezoelectric con-

Fig. 4. Linear intersubband optical absorption coefﬁcient a versus photon energy in an In0:4 Ga0:6 N=Al0:7 Ga0:3 N quantum well with the well width L ¼ 6 nm. Here the electron density is chosen as 5:0 1018 cm3 and T ¼ 300 K.

stants are e31 ¼ 0:2ð1 xÞ 0:23x C=m2 and e33 ¼ 0:29ð1 xÞ þ 0:39x C=m2 [23]. The elastic constants are C 13 ¼ 11:4ð1 xÞ þ 9:4x and C 33 ¼ 38:1ð1 xÞ þ 20:0x in units of 1011 dyn=cm2 [24]. The relaxation time is tin ¼ 0:24 ps [25]. In order to understand the following results, we should note that, in Section 2, the BEF F has been deﬁned as an electric ﬁeld induced by the spontaneous polarization of the wurtzite structure and the piezoelectric polarization due to the lattice mismatch between the Inx Ga1x N and Aly Ga1y N layers. Hence the F is not obviously inﬂuenced by the electronic charge redistribution or accumulation in the QW. Moreover, following Refs. [18,20,26], the inﬂuence of the electronic charge accumulation in the QW on the electron energy level distribution is minor and has been ignored in the present calculations. Fig. 3 shows our theoretical results of the absorption coefﬁcient a for three different optical intensities. Based on Eq. (20), we can see that the saturated absorption occurs at I ¼ 25 MW=cm2 . Considering the BEF effect, we calculate the linear absorption coefﬁcient in Fig. 4. For comparison, the result without the BEF effect is also given in Fig. 4. We can easily ﬁnd that the absorption peak is shifted to a higher energy due to the BEF. The shift of the absorption peak can be explained based on

Fig. 3. Intersubband optical absorption coefﬁcient a for an In0:3 Ga0:7 N=Al0:6 Ga0:4 N quantum well with the well width L ¼ 6 nm for three different optical intensities: (i) I ¼ 0, (ii) I ¼ 15 MW=cm2 , and (iii) I ¼ 25 MW=cm2 . Here the built-in electric ﬁeld is considered. The electron density is chosen as 5:0 1018 cm3 and T ¼ 300 K.

Fig. 5. Linear intersubband optical absorption coefﬁcient a as a function of the photon wavelength in Inx Ga1x N=Al0:6 Ga0:4 N QWs with the well width L ¼ 6 nm. Here the built-in electric ﬁeld is included. The electron density is chosen as 5:0 1018 cm3 and T ¼ 300 K. Five different In compositions are considered: (i) x ¼ 0:30, (ii) x ¼ 0:35, (iii) x ¼ 0:40, (iv) x ¼ 0:45, and (v) x ¼ 0:50.

the quantum conﬁned Stark effect induced by the BEF (refer to Fig. 2). In order to investigate the inﬂuence of the well depth on the intersubband optical absorption, we calculate the linear absorption coefﬁcient for different In (Al) fraction x (y) in the Inx Ga1x N/Aly Ga1y N strained single QWs. We can ﬁnd from Figs. 5 and 6 that the peak wavelength of the intersubband optical absorptions decreases if the In (Al) composition increases. The physical reason can be understood as follows. If In fraction x increases, the BEF becomes much stronger (refer to Fig. 1) and the potential well is much deeper. The energy difference between the two conﬁned electron states increases. If Al composition y increases, the QW depth becomes much deeper. Similarly, the energy difference between the two conﬁned electron states becomes larger. The absorption peak will thus be moved to a higher energy. The results of Figs. 5 and 6 are useful for designing electro-optical modulators and photodetectors in the near-infrared region. Fig. 7 indicates the calculated linear absorption coefﬁcient a for the In0:3 Ga0:7 N=Al0:6 Ga0:4 N QW with different electron concentrations. We can ﬁnd from Fig. 7 that the value of the absorption peak is enhanced if the electron density increases. This can be

ARTICLE IN PRESS 1840

Y.-m. Chi, J.-j. Shi / Journal of Luminescence 128 (2008) 1836–1840

layers. We ﬁnd that the BEF is very strong, of the order of MV/cm. The increase of the In composition will enhance the strength of the BEF. Considering the strong BEF effect, we further calculate the linear and nonlinear intersubband optical absorption coefﬁcients by using the density matrix method. Our results show that the position of the absorption peak has a great blue shift due to the strong BEF. Moreover, we ﬁnd that the saturated absorption can be obtained when I ¼ 25 MW=cm2 for an In0:3 Ga0:7 N=Al0:6 Ga0:4 N QW with the well width L ¼ 6 nm if choosing electron density as 5:0 1018 cm3 and T ¼ 300 K. The increase of the compositions of In and Al reduces the peak absorption wavelength. The magnitude of the optical absorption coefﬁcient increases if the electron density increases. Based on the present results, we hope that the important infrared photodetectors and nearinfrared laser ampliﬁers can be constructed based on the groupIII nitride QWs. Fig. 6. Linear intersubband optical absorption coefﬁcient a as a function of the photon wavelength in In0:3 Ga0:7 N=Aly Ga1y N QWs with the well width L ¼ 6 nm. Here the built-in electric ﬁeld is included. The electron density is chosen as 5:0 1018 cm3 and T ¼ 300 K. Five different Al compositions are considered: (i) y ¼ 0:60, (ii) y ¼ 0:65, (iii) y ¼ 0:70, (iv) y ¼ 0:75, and (v) y ¼ 0:80.

Acknowledgments This work was funded jointly by the National Basic Research Program of China under Grant no. 2006CB921607 and the China-Australia special fund of the National Natural Science Foundation of China for science and technology under Grant no. 60711120203. References

Fig. 7. Linear intersubband optical absorption coefﬁcient a as a function of the photon wavelength in an In0:3 Ga0:7 N=Al0:6 Ga0:4 N QW with the well width L ¼ 6 nm at T ¼ 300 K. Here the built-in electric ﬁeld is considered. Three different electron densities are chosen: (i) 3:0 1018 cm3 , (ii) 7:0 1018 cm3 , and (iii) 1:0 1019 cm3 .

completely understood based on Eqs. (5) and (16). The physical reason is because the Fermi level increases with the electron density increasing. The matrix element jM21 j and the initial (ﬁnal) state energy E1 (E2 ) are invariable due to a constant BEF F (see the above analysis). Hence the magnitude of the absorption peak should increase if increasing the electron density, as shown in Fig. 7.

6. Conclusions In conclusion, we have calculated the BEF in wurtzite Inx Ga1x N/Aly Ga1y N strained single QWs with a thin Inx Ga1x N strained layer sandwiched between the two thick Aly Ga1y N

[1] S. Nakamura, M. Senoh, S. Nagahama, N. Iwasa, T. Yamada, T. Matsushita, H. Kiyoku, Y. Sugimoto, T. Kozaki, H. Umemoto, M. Sano, K. Chocho, Appl. Phys. Lett. 73 (1998) 832. [2] S. Nakamura, S.F. Chichibu, Introduction to Nitride Semiconductor Blue Lasers and Light Emitting Diodes, Taylor & Francis, London, 2000. [3] C. Gmachl, H.M. Ng, A.Y. Cho, Appl. Phys. Lett. 77 (2000) 334. [4] D. Hofstetter, L. Diehl, J. Faist, W.J. Schaff, J. Hwang, L.F. Eastman, C. Zellweger, Appl. Phys. Lett. 80 (2002) 2991. [5] B.K. Ridley, W.J. Schaff, L.F. Eastman, J. Appl. Phys. 94 (2003) 3972. [6] M. Tchernycheva, L. Nevou, L. Doyennette, F.H. Julien, E. Warde, F. Guillot, E. Monroy, E. Bellet-Amalric, T. Remmele, M. Albrecht, Phys. Rev. B 73 (2006) 125347. [7] C. Gmachl, H.M. Ng, S.-N.G. Chu, Appl. Phys. Lett. 77 (2000) 3722. [8] N. Iizuka, K. Kaneko, N. Suzuki, T. Asano, S. Noda, O. Wada, Appl. Phys. Lett. 77 (2000) 648. [9] N. Iizuka, K. Kaneko, N. Suzuki, Appl. Phys. Lett. 81 (2002) 1803. [10] S.Y. Lei, B. Shen, L. Cao, F.J. Xu, Z.J. Yang, K. Xu, G.Y. Zhang, J. Appl. Phys. 99 (2006) 074501. ¨ nlu¨, I¨. Karabulut, H. S- afak, Physica E 33 (2006) 319. [11] S. U [12] P. Waltereit, M.D. Craven, S.P. DenBaars, J.S. Speck, J. Appl. Phys. 92 (2002) 456. [13] F. Bernardini, V. Fiorentini, D. Vanderbilt, Phys. Rev. Lett. 79 (1997) 3958. [14] J.J. Shi, Solid State Commun. 124 (2002) 341. [15] V. Jovanovic´, D. Indjin, Z. Ikonic´, V. Milanovic´, J. Radovanovic´, Solid State Commun. 121 (2002) 619. [16] F. Bernardini, V. Fiorentini, D. Vanderbilt, Phys. Rev. B 56 (1997) R10024. [17] T. Takeuchi, S. Sota, M. Katsuragawa, M. Komori, H. Takeuchi, H. Amano, I. Akasaki, Jpn. J. Appl. Phys. 36 (Part 2) (1997) L382. [18] S.H. Pan, S.M. Feng, Phys. Rev. B 44 (1991) 8165. [19] J.J. Shi, E.M. Goldys, IEEE Trans. Electron Devices 46 (1999) 83. ¨ . Atav, H. S- afak, M. Tomak, Eur. Phys. J. B 55 (2007) 283. [20] I˙. Karabulut, U [21] T. Takeuchi, H. Amano, I. Akasaki, Jpn. J. Appl. Phys. 39 (Part 1) (2000) L413. [22] I. Vurgaftman, J.R. Meyer, L.R. Ram-Mohan, Appl. Phys. Lett. 89 (2001) 5815. [23] T. Takeuchi, C. Wetzel, S. Yamaguchi, H. Sakai, H. Amano, I. Akasaki, Y. Kaneko, Y. Yamaoka, S. Nakagawa, N. Yamada, Appl. Phys. Lett. 73 (1998) 1691. [24] M. Yamaguchi, T. Yagi, T. Azuhata, T. Sota, K. Suzuki, S. Chichibu, S. Nakamura, J. Phys.: Condens. Matter 9 (1997) 241. [25] S.-H. Park, D. Ahn, E.H. Par, T.K. Yoo, Appl. Phys. Lett. 87 (2005) 044103. [26] D. Ahn, S.L. Chuang, IEEE J. Quantum Electron. QE-23 (1987) 2196.

Copyright © 2024 C.COEK.INFO. All rights reserved.